Polymer 46 (2005) 2452–2460
Photophysical study of a conjugated–non-conjugated PPV-type
A.M. Machadoa,b, J.D. Da Motta Netoa, R.F. Cossielloc, T.D.Z. Atvarsc, L. Dingd,
F.E. Karaszd, L. Akcelruda,*
´ ´ ´
Departamento de Quımica, Universidade Federal do Parana, Centro Politecnico, Caixa Postal 19081, 81531-990 Curitiba/PR, Brazil
Instituto Tecnologico para o Desenvolvimento LACTEC, Centro Politecnico, 81531-990 Curitiba/PR, Brazil
Instituto de Quımica, Universidade Estadual de Campinas, Caixa Postal 6154, 13084-971 Campinas/SP, Brazil
Department of Polymer Science and Engineering, University of Massachusetts, Amherst, MA 01003, USA
Received 4 November 2004; accepted 4 February 2005
This paper reports the photo- and electroluminescence studies of emitting species of one of the ﬁrst reported blue emitters, the conjugated–
non-conjugated multi-block copolymer, poly[1,8-octanedioxy-2,6-dimethoxy-1,4-phenylene-1,2-ethenylene-1,4-phenylene-1,2-ethenylene-
3,5-dimethoxy-1,4-phenylene]. Because the conjugation length of the emissive center is very well deﬁned (two and half phenylene–vinylene
units) the differences found between the ﬂuorescence proﬁle of the ﬂuorophore in solution, at several concentrations and that in the solid state
allowed us to conclude that in solid the emission comes from associated forms, such as ground-state dimers and/or excimers. Time-resolved
ﬂuorescence in a nanosecond time scale recorded at 6emZ24,096 cmK1 showed a monoexponential decay of 1.5 ns, which is compatible
with rigid forms of stilbene derivatives.
q 2005 Elsevier Ltd. All rights reserved.
Keywords: Electroluminescence; Photoluminescence; Conjugated–non-conjugated block copolymer
1. Introduction demonstrated that the device efﬁciency increases by up to
30 times in the prototypical polymer poly-(phenylene
Studies on copolymers in which a well-deﬁned emitting vinylene) (PPV)  with random interruption of conju-
unit is intercalated with non-emitting blocks have demon- gation by saturated groups in relation to the corresponding
strated that the emitted color is not affected by the PPV devices .
interspacer non-conjugated length. Nevertheless, the EL One of the ﬁrst reported conjugated–non-conjugated EL
efﬁciency of the single layer LEDs fabricated with this type copolymers was the blue emitter containing PPV type
of copolymer depends on the length of the non-conjugated blocks (2,1/2PPV units) interspersed among octamethylene
blocks: copolymers where longer spacers yielded higher- sequences, that is, poly[1,8-octanedioxy-2,6-dimethoxy-
efﬁciency devices [1–5]. Those conjugated–non-conjugated 1,4-phenylene-1,2-ethenylene-1,4-phenylene-1,2-etheny-
copolymers are soluble, uniform in terms of conjugation lene-3,5-dimethoxy-1,4-phenylene] , whose chemical
length and can be designed to emit in any portion of the structure is shown in Fig. 1. The EL properties of a device
visible spectrum [6–9]. For example, it has been produced with this material are well documented, but, to our
knowledge, the exact nature of the emitting centers has not
been explored. In this study we describe some results
* Corresponding author. Tel.: C55 413 367 507. obtained by dynamic ﬂuorescence decays and steady-state
E-mail address: firstname.lastname@example.org (L. Akcelrud). ﬂuorescence emission in an effort to identify the species
0032-3861/$ - see front matter q 2005 Elsevier Ltd. All rights reserved. responsible by the mechanism of photo- and electrolumi-
doi:10.1016/j.polymer.2005.02.007 nescence processes.
A.M. Machado et al. / Polymer 46 (2005) 2452–2460 2453
Fig. 1. Synthetic route and structures of dialdehyde and multi block conjugated–non-conjugated copolymer.
2. Experimental Dynamic ﬂuorescence decay, at room temperature, was
performed by single photon counting (Edinburgh Analytical
2.1. Materials nF900 system) operating with a pulsed hydrogen lamp at a
repetition rate of 40 kHz. The excitation wavenumber was
Dimethylformamide (Vetec, Brazil) was distilled under coincident with the excitation peak 6excZ27,027 cmK1 for
vacuum (5 mm Hg) and stored under molecular sieves the chromophoric block absorption. The emission wave-
(4 A). Ethanol was ﬁrstly reﬂuxed with CaO (Vetec, Brazil) number for the collection of counts was in the ﬂuorescence
during 24 h and after distilled. 3,5-dimethoxy-4-hydroxy- maximum 6emZ24,096 cmK1 (415 nm) for the chromo-
benzaldehyde (Aldrich), 1,9-dibromooctane (Aldrich), phoric block. The sample solutions were degassed and
p-xylene-bis(triphenylphosphonium bromide) (Aldrich), maintained in a sealed quartz tube. The sample ﬁlms were
metallic sodium, hydrochloric acid, iodine, sodium carbon- also degassed and sealed in a rectangular capilar. The
ate (Vetec, Brazil) were used without further puriﬁcation. instrument’s response was determined at every measure-
ment using Ludoxw as scatterer. At least 104 counts were
2.2. Monomer synthesis and polymerization collected in the peak channel. Deconvolution of the lamp
pulse was performed by nonlinear least-squares routines
The monomer synthesis was performed according to using the software supplied by Edinburg. The best ﬁt was
published procedures [2,8]. The polymer was prepared by achieved when the c2 is close to one and the residual
classical Wittig condensation . distribution is random.
2.3. Methods 2.3.3. FTIR and 1H and 13C NMR
The monomers and the polymer were characterized by
2.3.1. Molecular weight determination FTIR and NMR and the data are compared with the
A Waters gel permeation chromatograph equipped with literature. Samples for FTIR measurements were prepared
two columns HR4E and HR5E (polystyrene), pump model as KBr disks. Spectra were taken in a Bomem MB 100 FTIR
1500 was used. The solvent was DMF, in a ﬂux of Spectrophotometer, in the spectral range of 600–4,000 cmK1,
0.6 ml minK1, at 27 8C and the columns were connected to a with resolution of 2 cmK1, and 16 scans.
dual detector (UV, refraction index), and the calibration was A NMR Brucker 400 MHz Advance series with 13C at
based on PS standards. 100 MHz and 1H at 400 MHz equipment or an AC 200 MHz
Brucker with 13C at 50 MHz and 1H at 200 MHz were used.
2.3.2. Absorption and ﬂuorescence spectroscopies All NMR experiments used CDCl3 as a solvent and TMS as
A UV–Vis Shimadzu model NIR 3101 was used for the internal standard.
absorption measurements. Steady-state ﬂuorescence spec-
troscopy was performed in a ISS-PC1 spectroﬂuorimeter 2.3.4. Device fabrication
operating with a 300 W Xe arc lamp, with excitation Solutions of polymer (20 mg/ml in chloroform) were
wavenumber ca. 6excZ27,027 cmK1 (370 nm), collecting ﬁltered through 0.2 mm Millex-FGS Filters (Millipore Co.)
the emission from 6 emZ18,000–26,000 cmK1 (560– and were then spin coated onto PEDOT/Indium tin oxide
400 nm). In addition, excitation spectra were also recorded (ITO)-coated glass substrates (OFC Co.) under nitrogen.
from 6 excZ33,333–20,000 cmK1 (300–500 nm) with Calcium layer (thickness ca. 400 nm) was evaporated onto
6emZ22,831 cmK1 (438 nm). Emission and excitation the polymer at about 10K7 Torr, followed by a protective
spectra were performed with a triangular cuvette, as coating of aluminum. The devices were characterized using
recommended when concentrated solutions are analyzed, a system described elsewhere . PL measurements were
to minimize the inner ﬁlter effect. carried out using cast ﬁlms onto quartz surfaces ‘in situ’.
2454 A.M. Machado et al. / Polymer 46 (2005) 2452–2460
Fig. 2. 1H NMR and 13C NMR spectrum of dialdehyde and copolymer in CDCl3 solution; (a) 1H NMR of the dialdehyde; (b) 13C NMR of the dialdehyde; (c) 1H
NMR of the copolymer; (d) 13C NMR of the copolymer.
The thickness was adjusted in order to assure an optical the Fermi level in the reference determinant. For instance,
behavior according to Beer’s law. for the monomer one of the largest gaps in highest occupied
molecular orbitals (HOMOs) is 0.023 Hartree between MO
#101 and MO #102. One of the largest gaps in lowest
2.3.5. Quantum chemical calculations
unoccupied molecular orbitals (LUMOs) is 0.015 Hartree
Quantum chemical calculations have been carried out for
between MO #121 and MO #122. Therefore, the active
the monomer, dimer and trimer sequences. For each
space included all MOs between #102 and #121. We tried
oligomer, geometries have been fully optimized, using the
several variations in the size of the CI space, and the
AM1 Hamiltonian of Dewar and coworkers [13,14]. In this
resulting spectrum did not change except for a couple of
step, we have used the MOPAC code. Due to the large
wavenumbers. That suggests that our results are consistent.
number of atoms involved in the calculations, we have
All calculations have been carried out under FreeBSD
established a residual gradient norm of about 5.0 as a
reasonable ﬁgure. Optimization was carried out in Cartesian
coordinates (keyword XYZ), because optimization of
internal coordinates proved too difﬁcult to achieve. For
each optimized structure, electronic absorption spectra have
3. Results and discussion
been simulated with the INDO/S technique as suggested by
Zerner [15,16]: the reference determinant was obtained at
the self-consistent ﬁeld (SCF) level using the intermediate 3.1. Copolymer characterization
neglect of differential overlap (INDO/1) Hamiltonian, and
the electronic spectrum was obtained by a subsequent
Molecular weight was determined as M w Z 41 kg molK1
conﬁguration interaction (CI) calculation which included
and M n Z 29 kg molK1 with polydispersity index of ca. 1.44.
the reference determinant plus singly excitations only. The The copolymer’s structure was characterized by 1H NMR
usual routine in INDO/S calculations deﬁnes the CI active and 13C NMR spectra. Fig. 2 shows the assigned 1H NMR
space in terms of the energy separation between MOs near and 13C NMR spectra for the dialdehyde and copolymer.
A.M. Machado et al. / Polymer 46 (2005) 2452–2460 2455
Fig. 3. Normalized ﬂuorescence spectra of the copolymer in CHCl3 solutions,
6excZ27,027 cmK1 (370 nm). Concentrations: 10K6 mol lK1 (-x-x-), Fig. 5. Absorption spectrum of the copolymer in solution of CHCl3.
10K5 mol lK1 (—), 10K4 mol lK1 (- - -), 10K3 mol lK1 (-o-o-). Concentration: 10K5 mol lK1.
NMR and FTIR (not shown) results are consistent with observation can be explained by either the presence of the
those reported in the literature . inner ﬁlter effect with reabsorption of the higher energy
emission or by the formation of emitting aggregated species.
3.2. Emissive properties As we have employed a triangular cuvette, we have assumed
that although minimized, the inner effect could not be
Fig. 3 presents the ﬂuorescence spectra (6 excZ neglected. On the other hand, the presence of aggregates or
27,027 cmK1) of solutions of concentrations 10K3–10K6 associated polymer chains should increase the relative
mol lK1. Spectra of polymer solutions showed similar intensity of the red-edge, in addition to the decrease of the
proﬁles being composed by a broad band peaking at blue-edge, if there were ﬂuorescent, which was not the case.
6emZ23,094 cmK1 (433 nm) resulting from the overlap- This lead to the conclusion that in solution the aggregates
ping of vibronic bands, with a higher energy shoulder at exhibited a low ﬂuorescence quantum yield or were not
23,980 cmK1 (417 nm). Increasing the concentration up to present at all.
10K3 mol lK1 reduced the relative intensity of the blue-edge The excitation spectrum for all solutions, with 6emZ
of the emission band and the spectra became narrower. This 22,780 cmK1 are shown in Fig. 4. The spectra of the diluted
Fig. 4. Fluorescence (6excZ27,027 cmK1) (370 nm) (—) and excitation (6emZ22,780 cmK1) (439 nm) (- - -) spectra of the copolymer in solutions of CHCl3:
(a) 10K6 mol lK1, (b) 10K5 mol lK1, (c) 10K4 mol lK1, (d) 10K3 mol lK1.
2456 A.M. Machado et al. / Polymer 46 (2005) 2452–2460
the two dipole moments of the molecules in the dimer is
parallel and with opposite direction . This exciton
splitting in the range of 1,200–3,000 cmK1 is similar to that
of small molecules and is compatible with an interplanar
distance of 3–5 A [19,20].
The photoluminescence quantum yield of the copolymer
in diluted solutions (measured with 9,10-diphenylanthra-
cene as standard)  was 4FZ0.35, substantially higher
than that of trans-stilbene, 4FZ0.07 in the same solvent.
Fig. 6. Exciton splitting for a dimer compared to the isolated lumophore.
2 B is the Davidov splitting.
This could be explained by the increase in the rigidity and
planarity of the polymer-tied chromophore in relation to the
solutions 10K6 and 10K5 mol lK1 (Fig. 4(a) and (b)) were ‘free’ stilbene. Longer lifetime of stilbene derivatives were
similar to the absorption spectrum (Fig. 5), the band is attributed to the increase of their structural rigidity (i.e.
centered at 6excZ27,027 cmK1 (370 nm) with a shoulder at more rigid forms have higher quantum yields and also
25,580 cmK1 (390 nm) and were the mirror image of the longer lifetimes) .
emission spectrum at the same concentration, with a large The ﬂuorescence lifetime for the copolymer measured in
Stokes shift (6excK6emz3,933 cmK1). This behavior is 10K3 M chloroform solutions, was 1.19–1.20 ns, (Fig. 7).
characteristic of the emission of an isolated chromophore, Under the instrumental conditions employed here only
the conjugated segment corresponding to two and half decays longer than 0.5 ns could be recorded. Experimental
phenylene vinylene units, in this case. curve proﬁle can be ﬁtted using a monoexponential
The excitation spectra of concentrated solutions (10K4 M function, with c2Z0.991 and good residual random
and 10K3 mol lK1, Fig. 4(c) and (d)), however, are split into distribution, but the existence of lifetimes faster than
0.5 ns cannot be excluded. Reported lifetimes for stilbene
two bands at6excZ25,125 and 26,525 cmK1. Since the
and stilbene derivatives have been extensively explored in
emission spectra were centered at 6emZ22,935 cmK1 (Fig.
the literature [21,22] but an unquestionable agreement is
3), a smaller Stokes shift (6excK6emz 3190 cmK1) was
still needed. Lifetimes spanning from 0.14 to 1.8 ns, with
obtained. Simultaneous changes of both excitation and
mono and bi-exponential decays have been found [23,24].
emission spectra, recorded under conditions that minimize
Different emission mechanisms have been also proposed. In
the inner effect, are usually attributed to the excitonic
some cases monoexponential decay is suggested 
splitting observed when ground state dimers are formed
whereas others defend a biexponential decay . Accord-
. Similar results have already been obtained with ing to our data and with the higher value for the quantum
substituted stilbenes . yield for the copolymer in solution, the longer observed
Assuming that the splitting of the excitation bands were decay ca. 1.20 ns is explained by the larger rigidity of the
originated from dimer by an excitonic effect, the Davidov polymer chain compared to the free lumophore. As the
splitting energy (2 B)  could be estimated from the temporal resolution of our instrument does not cover
difference between the excitation maximum of the isolated the pico-second scale, excitation with other wavelengths
chain in diluted solution (6excZ27,027 cmK1) (Fig. 4(a)) was not done, since that will not add more information about
and the excitation maximum of split peak in concentrated the aggregation state of the emitting center.
solution (6excZ25,125 cmK1) (Fig. 4(d)) as being ca. The proﬁle of the ﬂuorescence band (PL) of the
1,902 cmK1. For illustration, see scheme in Fig. 6. The red- copolymer in the solid state, shown in Fig. 8, is red-shifted
shift of the excitation spectra suggests, according to the (6emZ22,124 cmK1) in relation to the spectrum of the
same exciton splitting model, that the relative orientation of polymer in chloroform diluted (Fig. 4(a)) (6 em Z
23,094 cmK1) and concentrated (Fig. 4(d)) solutions
(6emZ22,935 cmK1). Red-shift of the emission band of
conjugated polymers in solid state compared with solutions
can be attributed to several factors: increase of the critical
conjugation length; energy transfer processes from shorter
to longer chains; presence of associated interchain species in
the electronic ground state (dimers) or in the electronic
excited state (excimers) [26–32]. Considering that the
conjugation length of this PPV-type copolymer is deﬁned
by its chemical structure and no further increase of the
length can be imposed by the rigidity of the medium, the
Fig. 7. Fluorescence decay of the copolymer (10K3 M in CHCl3). 6emZ spectral red-shift must be attributed to the presence of
22,883 cmK1 (437 nm), 6excZ27,027 cmK1 (370 nm). This includes: lamp associated interchain species (dimer or excimer). The
proﬁle and the superimposed best ﬁt to the experimental data. vibronic structure of the PL spectrum evidenced by the
A.M. Machado et al. / Polymer 46 (2005) 2452–2460 2457
Fig. 8. Photoluminescence (—) and electroluminescence (-x-x-) spectra. EL device: (ITO/PEDOT/copolymer/Ca).
shoulder at 21,053 cmK1 suggests that the ground state state are expected to be similar. However, if excitonic decay
dimer is the most probable associated species. is faster, and recombination is slower than the average
Differently, the electroluminescence spectrum is cen- polymer relaxation time, these two emissions can be distinct
tered at 6emZ21,186 cmK1, coincident with the vibronic as is the case observed here.
shoulder of the PL spectrum. Although we could explain the Taking into account the results presented so far
differences between the PL and the EL considering that the (steady state ﬂuorescence spectra, excitation spectra and
EL is usually generated near the Ca (opaque electrode) and ﬂuorescence decays), we propose that the blue emitting
to be detected should travel throughout the ﬁlm thickness, species in either in PL or in electroluminescent devices
increasing the probability of being partially self-absorbed, of poly[1,8-octanedioxy-2,6-dimethoxy-1,4-phenylene-1,2-
we consider that this possibility does not play an important ethenylene-1,4-phenylene-1,2-ethenylene-3,5-dimethoxy-
role because we are working with very thin ﬁlms. In 1,4-phenylene] are the ground state dimers and
addition, inner effect and radiative energy transfer processes aggregates in the solid state. Since excimers cannot be
should decrease the intensity at the blue-edge of the directly excited, they cannot be observed by excitation
emission band, which has not been observed. We suggest spectroscopy and although their formation could not be
that the red shift of the EL spectrum compared to the PL detected, their occurrence evidently cannot be discarded.
spectrum is related to the different emission zone in the thin We have already shown  that polar substituents bring
ﬁlms. The injected charge carriers may recombine and give about a strong tendency of aggregation in stilbene
rise to radiative emission in the area close to the polymer/Ca derivatives, red-shifting the emission . As with other
interface due to the unbalanced double injection possibly substituents, the four methoxy-groups in the aromatic rings
occurring in the devices. The tailing in the long wavelength of the conjugated segment of that polymer are probably
region is largely due to defects in the emissive polymer acting in same direction, increasing the probability of
layer which act as new recombination centers in which aggregation. In addition, the inter-chain interaction and the
excitons radiatively decay giving emissions different from creation of new excited state species has been the subject in
those from the pristine polymer backbone [33–35]. recent proposals from the spectroscopic data, mainly related
However, this is not the only reason for the differences to PPV [12,36], and PPV derivatives, such as poly(2-
between EL and PL spectra in the solid state. It is well methoxy-1,4 PPV) (MEH-PPV) [12,37] CN-PPV [38–40],
known that the fundamental mechanisms generating the poly(p-pyridyl vinylene) [41,42], acetoxy-PPV  and
excitonic states in the EL (charge recombination) or PL other light-emitting polymers [44–46] leading to evidences
(direct excitation) processes differ. The chain segments that interchain excitations play a signiﬁcant role in the
involved in these distinct processes may also differ. When emission processes.
an excitonic species is formed the environment surrounding
these segments has to relax to stabilize the new dipolar 3.3. Quantum chemical calculations
orientation. If both recombination and emission processes
are either faster or slower than the reorientation process then Energies of the several molecular orbitals have been
the EL and PL emanations from a relaxed Franck–Condon determined for the optimized geometry of the monomer,
2458 A.M. Machado et al. / Polymer 46 (2005) 2452–2460
Fig. 9. Optimized AM1 geometry of the isolated trimer.
Fig. 10. Optimized AM1 geometry of the two associated trimers.
INDO/S calculated absorption spectrum for the trimer, dimer and monomer of the isolated molecules
CI vector Trimer Dimer Monomer
n (cm )
Gosc. n (cmK1
) Gosc. n (cmK1) Gosc.
2 28,742 2.5230 28,851 0.0003 28,433 0.0004
3 29,520 1.7080 31,746 0.5226 28,851 0.0003
4 33,242 1.2363 32,235 0.8890 31,746 0.5226
5 35,554 0.0072 32,618 0.0027 32,235 0.8890
6 36,047 0.0199 34,733 0.0005 32,618 0.0027
7 38,082 0.3333 37,791 0.2186 34,733 0.0005
8 38,286 0.2036 39,991 0.1016 37,791 0.2186
9 38,525 0.1997 41,961 0.1838 39,991 0.1016
10 38,751 0.1935 43,439 0.1987 41,961 0.1838
11 39,097 0.5828 28,433 0.0004 43,439 0.1987
A.M. Machado et al. / Polymer 46 (2005) 2452–2460 2459
Summary of quantum chemical calculations. Transition energy, g (from AM1 optimization) and transition assignments (from INDO/S) for monomer, dimer,
trimer forms and the dimeric form of the trimer. NBFZnumber of basis functions
Oligomer NBF jj~ jj
S0/S1 (cmK1) (nm) S0/S3 (cmK1) (nm)
Monomer 208 2.66 28,090 (352) vw 29,032 (310) s
Dimer 408 2.86 29,070 (344) s 32,362 (309) s
Trimer 608 4.64 28,736 (348) s 33,223 (301) s
(Trimer)2 1216 4.82 29,763 (336) w 31,348 (319) s
dimer and trimer forms (Fig. 9) of the isolated molecules. copolymer in concentrated conditions (concentrated sol-
The transition energies for the electronic absorption spectra utions and solid state) was assigned to the ﬂuorescence of
were determined using the well known formula 1;3 associated forms, ca. ground state dimers or excimers, based
EZ 3i K 3a C Jia GKia [15,16]. We have also calculated on previous results obtained with substituted stilbenes. The
the oscillator strengths for each transition. Data are presence of the former was conﬁrmed by excitation spectra
summarized in Table 1. Usually, conﬁguration interaction and results from an intermolecular association, since it they
(CI) calculations for conjugated polymer systems present CI were seen only in concentrated conditions.
vectors with large mixing. In particular, for this copolymer The PL of the copolymer ﬁlms is redshifted in relation to
the calculated absorption spectra show an increasing the concentrated solution spectrum with 6emZ22,222 cmK1
resolution with the size of the polymer segment. For (450 nm) and a shoulder at 6emZ21,053 cmK1 (475 nm).
example, the spectrum of the monomer (Table 1) shows the The electroluminescence spectrum peaks at 21,053 cmK1,
expected large CI mixing, although it is still possible to indicating that the electroluminescence is originated from
obtain an approximate one electron picture for the spectrum. the aggregates, that absorbed directly the excitation or were
Among the three segments, the one composed by two mers excited through energy transfer from the excited state of the
(dimer) presents the calculated INDO/S spectrum with the isolated absorber. Both the substantially higher measured
closest resemblance to the experimental UV–visible spec- quantum yield and the longer monoexponential lifetime of
trum obtained in chloroform (Fig. 5). This calculated the copolymer compared to stilbene agree with the greater
spectrum is composed by two transitions at the same region: rigidity and planarity of the polymer-tied chromophore in
one low lying at 29,070 cmK1 and one higher energy at comparison with the free stilbene lumophore. To our
23,620 cmK1 (Table 2). Finally, it is easy to trace the knowledge, the lifetime for stilbene containing polymers
character of each transition down to a single excitation is reported for the ﬁrst time. Increase in planarity and
which in the case of the trimer can be assigned to the S0/ rigidity favors the aggregation processes.
S1 p,p* transition. In all spectra we obtained a quite simple
description in terms of an electron ‘jump’ between neighbor-
ing rings. Most transitions consist of excitations from an Acknowledgements
occupied p orbital ‘localized’ in a 2,5-dimethoxy-phenoxy
moiety to an unoccupied p* orbital of a phenyl ring in the next T.D.Z.A. and R.F.C. thank FAPESP, CNPq, FAEP/Uni-
neighboring monomeric unit. The proﬁle of the MOs involved camp and MCT/PADCT/IMMMP for ﬁnancial support and
in each transition suggests that all excitations tend to transfer fellowships. L.A. and A.M.M thank LACTEC, CNPq and
the electron from the middle towards the end of the segment. IMMP for ﬁnancial support. FEK thanks AFOSR for their
As an attempt to represent the absorption spectrum of support.
aggregates we simulate the spectrum of a p stack of two
segments of the trimer, whose geometry has also been
optimized (Fig. 10). The calculated interplanar distance of References
species is ca. 4.7 A. Interestingly enough, this distance was
maintained during a full geometry optimization (not even  Akcelrud L. Prog Polym Sci 2003;28:875.
symmetry constraints were imposed), suggesting that this  Yang Z, Sokolik I, Karasz FE. Macromolecules 1993;26:1188.
 Yang Z, Hu B, Karasz FE. Macromolecules 1995;28:6151.
association is remarkably stable. This distance is also in
 Kim DY, Cho HN, Kim CY. Prog Polym Sci 2000;25:1089.
agreement with the experimental data from the Davidov  Hu B, E F. Karasz. Chem Phys 1998;227:263.
splitting (3–5 A).  Yang Z, Hu B, Karasz FE. J Macromol Sci, Pure Appl Chem 1998;
 Hu B, Yang Z, Karasz FE. J Appl Phys 1994;76:2419.
 Sokolik I, Yang Z, Morton DC, Karasz FE. J Appl Phys 1993;74:3584.
 Hu B, Morton DC, Sokolik I, Yang Z, Karasz FE. J Lumin 1994;
4. Conclusions 60/61:919.
 Burn PL, Holmes AB, Kraft A, Brown AR, Bradley DDC, Friend RH.
The excitonic splitting found in the emission of the Mater Res Soc Symp Proc 1992;247:647.
2460 A.M. Machado et al. / Polymer 46 (2005) 2452–2460
 Zhang C, Braun D, Heeger AJ. J Appl Phys 1993;73:5177.  Von Seggern H, Wnkel PS, Zhang C, Schimdt HW. Macromol J Chem
 Hsu JWP, Yan M, Jedju TM, Rothberg LJ, Hsieh BR. Phys Rev B Phys 1994;195:2023.
1994;49:712.  Zheng S, Shi J, Mateu R. Chem Mater 2000;12:1814.
 Dewar MJS, Zoebisch EG, Healy EF, Stewart JJP. J Am Chem Soc  Yang Z, Hu B, Karasz FE. J Macromol Sci, Pure Appl Chem 1998;
 Dewar MJS, Zoebisch EG. J Mol Struct Theochem 1988;180.  Burn PL, Holmes AB, Kraft A, Bradley DDC, Brown AR, Friend RH,
 Ridley JE, Zerner MC. Theoret Chim Acta (Berlin) 1973;32:111. Gymer RW. Nature 1992;356(6364):47.
 Zerner MC, Low GH, Kirchner RF, Mueller UT. Westerhoff. J Am  Zheng M, Ding L, Karasz FE. Macromol Chem Phys 2002;203:1337.
Chem Soc 1980;102:589.  Zheng M, Ding L, Lin Z, Karasz FE. Macromolecules 2002;35:9939.
 Lackowicz JR. Principles of ﬂuorescence spectroscopy. 2nd ed. New  Chu Q, Pang Y, Ding L, Karasz FE. Macromolecules 2002;35:7569.
York: Kluwer Academic Publishers; 1999.  Rothberg LJ, Yan M, Papadimitrakopoulos F, Galvin ME,
 Aguiar M, Pinto MR, Atvars TDZ, Akcelrud L, Saltiel J. J Photosci Kwock FW, Miller TM. Synth. Met 1996;80:41.
 Cossiello RF, Akcelrud L, Atvars TDZ. J Braz Chem Soc. 2005;16:74.
 Kasha M, Rawls HR, El-Bayoumi MA. Pure Appl Chem 1965;11:371.
 Conwell E. Phys Rev B 1997;57:218.
 Bortolato CA, Atvars TDZ, Dibbern-Brunelli D. J Photochem
 Wu MW, Conwell E. Phys Rev B 1997;56:R10060.
Photobiol A: Chem 1991;59:123.
 Samuel ID, Rumbles G, Collison CJ. Phys Rev B 1995;51:R11573.
 Birch DJ, Birks JB. Chem Phys Lett 1976;38:432.
 Kakubiak R, Rothberg LJ, Wan W, Hsieh BR. Synth Met 1999;101:
 Taylor JR, Adams MC, Sibbett W. Appl Phys Lett 1979;35:590.
 Pyun C-H, Lyle TA, Daube GH, Park S-M. Chem Phys Lett 1986;124:
48.  Blatchford JW, Gustafson TL, Epstein AJ, Vandenbout D, Kerimo A,
 Traylor JR, Adams MC, Sibbett W. J Photochem 1980;12:127. Higgins DA, et al. Phys Rev B 1996;54:R3683.
 Charlton JL, Saltiel J. J Phys Chem 1977;20:1940.  Aguiar M, Figihara MC, Hummelgen IA, Peres LO, Garcia JR,
 Woo HS, Lhost O, Graham SC, Bredas JL, Schenk R, Mullen K. Synth Gruber J, et al. J Lumin 2002;96:219.
 Jenekhe AS, A Osaheni J. Science 1994;265(5173):765.
 Tian B, Zerbi G, Schenk R, Mullen K. J Chem Phys 1991;95:3191.  Aguiar M, Karasz FE, Akcelrud L. Macromolecules 1995;28:4598.
 Ohnishi T, Doi S, Tsuchida Y, Noguchi T. IEEE Trans Electron  Martin SJ, Cadby AJ, Lane PA, Bradley DDC. Synth Met 1999;101:
Devices 1997;44:1253. 665.